Jan 08, 2016 · EN 10083-3:2006 Steels for quenching and tempering. Technical delivery conditions for alloy steels:EN 10132-3:2000 Cold rolled narrow steel strip for heat treatment. Technical delivery conditions. Steels for quenching and tempering:EN 10263-4:2001 Steel rod, bars and wire for cold heading and cold extrusion. 34CrMo4 / 1.7220 - Steel NumberEN 10083-3:2006 Steels for quenching and tempering. Technical delivery conditions for alloy steels:EN 10132-3:2000 Cold rolled narrow steel strip for heat treatment. Technical delivery conditions. Steels for quenching and tempering:EN 10263-4:2001 Steel rod, bars and wire for
42CrMo4 is a steel for quenching and tempering, which has a good combination of strength and toughness in the quenched and tempered condition. After the oil quenching, the steel will be through hardened up to ø60 mm bar diameter. The microstructure of larger dimensions is not fully martensite. The steel is applicable to induction hardening. 42CrMo4 Steel Round Bar / Plate 1.7225 -EN 10083 - OATI First quenching heated slowly to 880°C, Then after adequate soaking at this temperature quench in oil or water. Temper as soon as tools reach room temperature. Second quenching heat to 780-820°C then quenching in oil or water. Tempering of 42CrMo4 Alloy structural steel; Heat to 205-649°C, then cool in water or oil. normal delivery AISI 4130 Steel - 25CrMo4 - JIS SCM430 - GB 30CrMo Heat to 900º C (1650 º F). Cool 4130 steel in air. Actually, when forgings are normalized before, say, carburizing or hardening and tempering, the upper range of normalizing temperatures is used. When normalizing is the final heat treatment, the lower temperature range is used. Hardening. Austenitize at 870º C (1600 º F), and quench in oil.
27MnCrB5 1.7182 (EN 10083-3) 30MnB5 1.5531 (EN 10083-3) 40MnB4 1.5527 Steels for quenching and tempering - with Cr and Mo GRADE W.Nr. + STANDARD 25CrMo4 1.7218 (EN 10083-3,EN10132-3) 34CrMo4 1.7220 42CrMo4 1.7225 42CrMoS4 1.7227 (EN 10083-3) 50CrMo4 1.7228 (EN 10083-3) 34CrMo44 1.7341 Steels for quenching and tempering - DIN EN 10083-1 Steels for quenching and tempering of EN 10083-2 and EN 10083-3 and in one of the surface conditions given in the relevant tables of EN 10083-2 and EN 10083-3. The steels are generally intended for the manufacture of quenched and tempered, flame or induction hardened machine parts, but can also be used in the normalized condition (see EN 10083-2). DIN1.7220 34CrMo4 Quenching and Tempering Steel - Tool Apr 07, 2016 · DIN1.7220 34CrMo4 Quenching and Tempering Steel Similar Grade:DIN1.7220 34CrMo4 Standard:EN10083-3 (Technical delivery conditions for Alloy steels in the quenched and tempered condition) Shape:round, flat, square. Size Range:Round :Diameter(mm):1.0-1000,
34CrMoS4 grade steel belongs to alloy steels for quenching and tempering. The material no. is 1.7226. Shanghai Katalor Industry Co., Ltd could supply the 34CrMoS4 steel plates, 34CrMoS4 steel sheets, 34CrMoS4 bars, 34CrMoS4 steel strips.We are always responsible for our customers and provide the best quality products. Hot rolled steels for quenching and tempering - alloy steelHot rolled steels for quenching and tempering alloy steelaccording DIN EN 10083-3. Our product portfolio also includes hot-rolled boron-alloyed tempered steel according to DIN EN 10083-3. Underneath, the grades 22MnB5 to 40MnB5 are led. The boron-alloyed tempered steels belong to the MnB series based on DIN EN 10083, Part 3. en10083 3 42crmo4 quenching and tempering steel 42CrMo4 / 1.7225 - Steel Number. EN 10083-3 2006 Steels for quenching and tempering.Technical delivery conditions for alloy steels EN 10132-3 2000 Cold rolled narrow steel strip for heat treatment.Technical delivery conditions.Steels for quenching and tempering EN 10305-1 2010 Steel tubes for precision applications.Seamless cold drawn tubes
Product Details EN 10083-3 34CrMo4 (1.7220) steel has high static strength, high impact toughness and high fatigue limit. Compared with 40Cr steel, 34CrMo4 steel has higher harden-ability. 34CrMo4 steel has high creep strength in high temperature, and it can work in 500 temperature.